High temperature molecular-based phase transition compounds with tunable and switchable dielectric properties
Wan, Min; Wang, Yan-Ning; Liu, Jing-Yuan; Tong, Liang; Ye, Si-Yu; Li, Jun-Yi; Chen, Li-Zhuang; CrystEngComm 24 (2022) 782–787; doi:10.1039/D1CE01488A

data_7244200
_publ_section_title
;
 High temperature molecular-based phase transition compounds with tunable
 and switchable dielectric properties
;
_journal_issue                   4
_journal_name_full               CrystEngComm
_journal_page_first              782
_journal_page_last               787
_journal_paper_doi               10.1039/D1CE01488A
_journal_volume                  24
_journal_year                    2022
_chemical_formula_moiety         '2(O4 Re), C8 H17 F N2'
_chemical_formula_sum            'C8 H16 F N2 O8 Re2'
_chemical_formula_weight         659.63
_space_group_crystal_system      orthorhombic
_space_group_IT_number           61
_space_group_name_Hall           '-P 2ac 2ab'
_space_group_name_H-M_alt        'P b c a'
_atom_sites_solution_hydrogens   geom
_audit_creation_date             2021-06-20
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_audit_update_record
;
2021-08-29 deposited with the CCDC.	2021-12-28 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   10.1928(5)
_cell_length_b                   14.8794(6)
_cell_length_c                   19.0803(8)
_cell_measurement_reflns_used    21673
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.0
_cell_measurement_theta_min      2.65
_cell_volume                     2893.8(2)
_computing_cell_refinement       'SAINT V8.18C (?, 2016)'
_computing_data_reduction        'SAINT V8.18C (?, 2016)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_diffrn_ambient_temperature      296.15
_diffrn_measured_fraction_theta_full 0.971
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0399
_diffrn_reflns_av_unetI/netI     0.0219
_diffrn_reflns_Laue_measured_fraction_full 0.971
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            21673
_diffrn_reflns_point_group_measured_fraction_full 0.971
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         24.999
_diffrn_reflns_theta_min         2.647
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    16.768
_exptl_absorpt_correction_T_max  0.134
_exptl_absorpt_correction_T_min  0.061
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    3.028
_exptl_crystal_description       BLOCK
_exptl_crystal_F_000             2408
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.12
_refine_diff_density_max         0.681
_refine_diff_density_min         -0.636
_refine_diff_density_rms         0.116
_refine_ls_extinction_coef       0.00241(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.075
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     191
_refine_ls_number_reflns         2540
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.075
_refine_ls_R_factor_all          0.0201
_refine_ls_R_factor_gt           0.0159
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
;
 w=1/[\s^2^(Fo^2^)+(0.0090P)^2^+2.9462P]
 where P=(Fo^2^+2Fc^2^)/3
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0327
_refine_ls_wR_factor_ref         0.0338
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2254
_reflns_number_total             2540
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d1ce01488a2.cif
_cod_data_source_block           FEtdabcoReO4
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'MULTI-SCAN' was
changed to 'multi-scan' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 7556 2019-12-06 15:28:31Z antanas 

 Adding full bibliography for 7244198--7244201.cif.
;
_cod_database_code               7244200
_shelxl_version_number           2013-2
_shelx_estimated_absorpt_t_max   0.238
_shelx_estimated_absorpt_t_min   0.134
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H,H) groups, All N(H) groups
2.a Ternary CH refined with riding coordinates:
 N2(H2)
2.b Secondary CH2 refined with riding coordinates:
 C1(H1A,H1B), C2(H2A,H2B), C3(H3A,H3B), C4(H4A,H4B), C5(H5A,H5B), C6(H6A,H6B),
 C7(H7A,H7B), C8(H8A,H8B)
;
_shelx_res_checksum              98077
_olex2_submission_special_instructions 'No special instructions were received'